Article Removal of Arsenic(III) Ion from Aqueous Media Using Complex Nickel-Aluminum and Nickel-Aluminum-Zirconium Hydroxides
Fumihiko Ogata 1 , Noriaki Nagai 1, Megumu Toda 2, Masashi Otani 2, Chalermpong Saenjum 3,4 , Takehiro Nakamura 1 and Naohito Kawasaki 1,5,*
1 Faculty of Pharmacy, Kindai University, 3-4-1 Kowakae, Higashi-Osaka, Osaka 577-8502, Japan; [email protected] (F.O.); [email protected] (N.N.); [email protected] (T.N.) 2 Kansai Catalyst Co. Ltd., 1-3-13, Kashiwagi-cho, Sakai-ku, Sakai, Osaka 590-0837, Japan; [email protected] (M.T.); [email protected] (M.O.) 3 Faculty of Pharmacy, Chiang Mai University, Suthep Road, Muang District, Chiang Mai 50200, Thailand; [email protected] 4 Cluster of Excellence on Biodiversity-based Economics and Society (B.BES-CMU), Chiang Mai University, Suthep Road, Muang District, Chiang Mai 50200, Thailand 5 Antiaging Center, Kindai University, 3-4-1 Kowakae, Higashi-Osaka, Osaka 577-8502, Japan * Correspondence: [email protected]; Tel.: +81-6-4307-4012
Received: 12 May 2020; Accepted: 12 June 2020; Published: 14 June 2020
Abstract: The technology of wastewater treatment involving removal of heavy metals using complex metal hydroxides is reported. In this study, complex nickel-aluminum (NA11 and NA12) and nickel-aluminum-zirconium (NAZ1 and NAZ2) hydroxides were prepared for the removal of arsenite ions, As(III), from aqueous solution. The characteristics of each adsorbent were evaluated, and the adsorption capacity and adsorption mechanism were determined. The adsorption capacity of As(III) 1 1 on NAZ1 (15.3 mg g− ) was greater than that on NA11 (9.3 mg g− ). Coverage is directly related to the speciﬁc surface area with a correlation coeﬃcient of 0.921. Ion exchange involving sulfate ions in the interlayer of the adsorbent also plays a role in the mechanism of As(III) adsorption as demonstrated by correlation coeﬃcients of 0.797 and 0.944 for the NA11 and NAZ1, respectively. The results demonstrate the usefulness of NAZ1 in removing As(III) from aqueous media.
Keywords: complex nickel-aluminum-zirconium hydroxide; arsenic ion; adsorption
1. Introduction The United Nations has adopted 17 goals as part of its 2030 agenda to develop a sustainable future for all. Issues of clean water and sanitation (Goal No. 6) and undersea water (Goal No. 14) are particularly relevant to the development of an acceptable global water environment . Heavy metals and their compounds are useful in many areas of human endeavor . However, their excessive use leads to an increasing presence in aqueous environments . Arsenic (As) pollution in aquatic systems is a global issue owing to its high toxicity and chronic eﬀects on human health [4,5]. Arsenic pollution in drinking water is a major concern in developing countries. Previous studies have identiﬁed a relationship between arsenic exposure and diseases such as asthma and hyperglycemia [6,7]. Arsenic and inorganic arsenic compounds are classiﬁed as Group 1 human carcinogens by the International 1 Agency for Research on Cancer . The World Health Organization has established 0.01 mg L− as the maximum permissible arsenic content in potable water to protect human health . The predominant forms of inorganic arsenic in aquatic systems are As(V) (arsenate) and As(III) (arsenite). Arsenic is a ubiquitous element, occurring from natural sources (such as wearing of arsenic bearing minerals and
Water 2020, 12, 1697; doi:10.3390/w12061697 www.mdpi.com/journal/water Water 2020, 12, 1697 2 of 11 volcanic eruptions) and anthropogenic activities (such as mining, glassware production, dyes, drugs, and pesticide industries) [10–12]. As(III) is highly toxic, soluble, and mobile compared to As(V) [13,14]. Therefore, there is a need for simple, eﬃcient, and inexpensive techniques to remove As(III) from aquatic systems. Adsorption techniques using a variety of materials have been shown to be superior to conventional techniques such as precipitation, reverse osmosis, ﬁltration, and biological treatment for As(III) removal [2,15]. Complex metal hydroxides are useful adsorbents for the removal of heavy metals from aqueous systems [16,17]. A complex metal hydroxide, or layered double hydroxide, contains divalent and trivalent cations at the octahedral positions of brucite-like layers. Anions are incorporated in the interlayer region for charge neutrality [18,19]. Multi-metal hydroxides exhibit substantially diﬀerent physicochemical characteristics than their single-metal counter parts. Their properties depend on the identities and molar ratios of the constituent metals . Many researchers have reported As(III) removal using adsorbents such as a Mn-oxide-doped Al oxide , an iron-zirconium binary oxide , a calcined Mg-Fe-La hydrotalcite-like compound , a nickel-aluminum hydroxide , and an Fe-Mg type hydrotalcite . Incorporation of zirconium (Zr4+) into a complex metal hydroxide such as a Mg-Al-layered double hydroxide has recently been examined [22,23]. Incorporation increases the charge in the metal layer and promises to be an attractive means of generating unique physicochemical properties. Positively charged brucite-like sheets have been prepared containing Zr4+, which randomly occupies the octahedral holes in a close-packed conﬁguration of hydroxide ions . Adsorption of phosphate ion from aqueous media using the Zr4+-containing complex metal hydroxide has been reported [22,23]. However, there have been no reports regarding As(III) adsorption from aqueous media. Arsenic as As(V) (arsenate) or As(III) (arsenite) adopts chemical forms similar to those of phosphorus as P(V) (phosphate) or P(III) (phosphite). We previously reported that nickel-aluminum-zirconium hydroxide is useful in the removal of phosphate ions from an aqueous phase . This paper focuses on the relationship between As(III) adsorption and the complex nickel-aluminum and nickel-aluminum-zirconium hydroxides. The objectives of this work are to determine the physicochemical characteristics of complex nickel-aluminum and nickel-aluminum-zirconium hydroxides as a function of composition, to evaluate their ability to adsorb As(III) from aqueous media, and to investigate the mechanism of As(III) adsorption.
2. Materials and Methods
2.1. Materials and Chemicals Nickel-aluminum and nickel-aluminum-zirconium hydroxides of diﬀerent compositions were obtained from Kansai Catalyst Co., Ltd., Japan. Nickel-to-aluminum molar ratios of 1 and 0.5 are designated as NA11 and NA12, respectively. Nickel:aluminum:zirconium molar ratios of 0.9:1.0:0.09 and 0.9:0.2:0.09 are denoted as NAZ1 and NAZ2, respectively. Sulfate was included as an exchangeable anion in the interlayer of NA and NAZ. These materials were synthesized by the following method. Nickel(II) sulfate hexahydrate, aluminum sulfate octahydrate, and zirconium(IV) sulfate tetrahydrate were mixed with distilled water (230 g) at heating. The reaction mixture was added to the distilled water (400 g) at pH 9.0 for 800 rpm at 25 ◦C. The solution pH was adjusted using a 25% sodium hydroxide solution. After mixing for 2 h, the suspension was ﬁltered, washed, and dried at 110 ◦C for 12 h. Arsenic(III) standard solution (As(III), As2O3 and NaOH in water pH 5.0 with HCl), hydrochloric acid, and sodium hydroxide were purchased from FUJIFILM Wako Pure Chemical Co., Japan. The purity grade of all reagents was special grade and the quality of water (resistivity) was 18.2 MΩ cm at 25 C. · ◦ 2.2. Physicochemical Properties of Adsorbents The NA11, NA12, NAZ1, and NAZ2 adsorbents were characterized as follows. The morphologies and crystallinities of the adsorbents were determined by scanning electron microscopy with an SU1510 Water 2020, 12, 1697 3 of 11 instrument (Hitachi High-technologies Co., Tokyo, Japan) and a Mini Flex II X-ray diﬀraction analyzer (Rigaku Co., Tokyo, Japan), respectively. The surface area was determined by a speciﬁc surface analyzer N42-25E (Quantachrome Instruments Japan G.K., Kanagawa, Japan). Surface hydroxyl groups were assayed using the ﬂuoride-ion adsorption method . Brieﬂy, the adsorbent (0.125 g) was mixed with 1 1 a 0.01 mol L− NaF solution (50 mL) at pH 4.6. The solution pH was adjusted by 0.2 mol L− acetic acid 1 solution and 0.2 mol L− acetate buﬀer solution. The reaction mixture was shaken for 24 h at 100 rpm and 25 ◦C and ﬁltered through a 0.45-µm membrane ﬁlter. The concentration of ﬂuoride ion before and after adsorption was measured using absorption spectrophotometry (DR890, HACH, Loveland, CO, USA). The amount of ﬂuoride ion adsorbed was calculated (the ratio of the concentration of ﬂuoride ion and the concentration of hydroxyl group is 1:1). The surface pH of the adsorbent was measured as follows. A 0.1-g quantity of adsorbent was added to 50 mL distilled water at pH 7.0. The suspension was shaken for 2 h at 100 rpm and 25 ◦C and ﬁltered through a 0.45-µm membrane ﬁlter. The solution pH was measured with a digital pH meter (F-73, Horiba, Ltd., Kyoto, Japan) .
2.3. Adsorption Experiments
1 NA11, NA12, NAZ1, and NAZ2 in 0.1-g quantities were mixed with 50 mL of 100 mg L− As(III) solution to determine the extent of As(III) adsorption. Mixtures were shaken for 24 h at 100 rpm and ﬁltered through a 0.45-µm membrane ﬁlter. The As(III) concentration of the ﬁltrate was measured by inductively coupled plasma optical emission spectrometry using an iCAP 7600 Duo instrument (ICP-OES, Thermo Fisher Scientiﬁc Inc., Kanagawa, Japan). The quantity of As(III) adsorbed was calculated from the diﬀerence in As(III) concentration before and after adsorption. To examine the 1 eﬀect of contact time, 0.1-g quantities of NA11 and NAZ1 were mixed with 50 mL of a 100 mg L− As(III) solution and shaken for 0.5, 1, 3, 6, 9, 12, 16, 20, and 24 h at 100 rpm and 25 ◦C. The eﬀect of pH 1 was studied by mixing the same adsorbents with 50 mL of 100 mg L− As(III) and adjusting the solution pH from 2 to 10 using hydrochloric acid or sodium hydroxide. The same adsorbents were mixed with 1 50 mL of 1, 10, 30, 50, 70, and 100 mg L− As(III) solutions to study the eﬀect of concentration. These solutions also were shaken for 24 h at 100 rpm and 25 ◦C. The quantity of sulfate ion released from adsorbent was measured to elucidate the adsorption mechanism of As(III). Sulfate ion concentration was determined by ion chromatography using a DIONEX ICS-900 instrument (Thermo Fisher Scientiﬁc Inc., Tokyo, Japan), an IonPac AS12A system (4 200 mm, Thermo × Fisher Scientiﬁc Inc., Tokyo, Japan), and an AMMS 300 (4 mm, Thermo Fisher Scientiﬁc Inc., Tokyo, 1 Japan) micro-membrane ﬁlter suppressor. The regenerant and mobile phase were 12.5 mmol L− 1 1 H2SO4, and 2.7 mmol L− Na2CO3 + 0.3 mmol L− NaHCO3, respectively. The ﬂow rate and sample 1 volume were 1.0 mL min− and 10 µL under ambient conditions. The quantity of sulfate ions released from adsorbent were calculated using the levels before and after adsorption in Equation (1):
q = (Ce C )V/W, (1) − 0 1 where q is the quantity of sulfate ion released (mg g− ); C0 is the concentration before adsorption 1 1 (mg L− ); Ce is the concentration after adsorption (mg L− ); V is the solvent volume (L); and W is the weight of the adsorbent (g). Data are presented as the mean standard deviation from 2–3 experiments. ± 3. Results and Discussion
3.1. Physicochemical Properties of Adsorbents The SEM images of each adsorbent are shown in Figure1. The adsorbents are not perfectly spherical in shape, but no signiﬁcant diﬀerences are observed in the appearance of the adsorbents in this study. Water 2020, 12, 1697 4 of 11 Water 2020, 12, x FOR PEER REVIEW 4 of 11 Water 2020, 12, x FOR PEER REVIEW 4 of 11
FigureFigure 1.1. SEM images of adsorbents. Figure 1. SEM images of adsorbents. FigureFigure2 2contains contains the the X-ray X-ray di ﬀ raction diffraction patterns. patterns. Peaks Peaks at (003), at (006), (003), (015), (006), and (015), (113) and are observed(113) are Figure 2 contains the X-ray diffraction patterns. Peaks at (003), (006), (015), and (113) are forobserved all adsorbents for all adsorbents indicating indicating that they that can they be indexed can be indexed to the crystal to the structurecrystal structure of the complexof the complex metal observed for all adsorbents indicating that they can be indexed to the crystal structure of the complex hydroxide.metal hydroxide. Peaks (003) Peaks and (003) (006) and are (006) attributed are attributed to basal reﬂections to basal reflectio that correspondns that correspond to the stacking to the of metal hydroxide. Peaks (003) and (006) are attributed to basal reflections that correspond to the thestacking brucite-like of the sheets brucite [-27like]. Some sheets NAZ . peaks Some are NAZ comparable peaks are to comparable those in NA, to which those in indicates NA, which that stacking of the brucite-like sheets . Some NAZ peaks are comparable to those in NA, which Zrindicates4+ has beenthat Zr successfully4+ has been incorporatedsuccessfully incorporated into the octahedral into the layeroctahedral of the layer complex of the nickel-aluminum complex nickel- indicates that Zr4+ has been successfully incorporated into the octahedral layer of the complex nickel- hydroxide.aluminum hydroxide. Zirconium(IV) Zirconium(IV) insertion alters insertion the distances alters the between distances metals between and metals between and the between octahedral the aluminum hydroxide. Zirconium(IV) insertion alters the distances between metals and between the layers.octahedral Similar layers. trends Similar have trends been reportedhave been in reported previous in investigations previous investigations [22,23]. [22,23]. octahedral layers. Similar trends have been reported in previous investigations [22,23].
Figure 2. XRD patterns of adsorbents. Figure 2. XRD patterns of adsorbents. Figure 2. XRD patterns of adsorbents. Some characteristics of the adsorbents are shown in Table1. Surface pH and the number of Some characteristics of the adsorbents are shown in Table 1. Surface pH and the number of hydroxylSome groups characteristics of NA are of higher the adsorbents than those are of shown NAZ. inHowever, Table 1. the Surface speciﬁc pH surface and the area number of NAZ of hydroxyl groups of NA are higher than those of NAZ. However, the specific2 1 surface area of NAZ is hydroxylis greater groups than that of NA of NA. are higher The speciﬁc than those surface of NAZ. area of However, NAZ1 (51.9 the mspecificg− ) surface is greater area than of NAZ that ofis greater than that of NA. The specific surface area of NAZ1 (51.9 m2 g−1) is greater than that of greater than that of NA. The specific surface area of NAZ1 (51.9 m2 g−1) is greater than that of previously reported (Mg(AlZr)-LDHs(CO3 or Cl) = 2.2–39 m2 g−1 and Zr-MgAl = 49 m2 g−1) adsorbents, previously reported (Mg(AlZr)-LDHs(CO3 or Cl) = 2.2–39 m2 g−1 and Zr-MgAl = 49 m2 g−1) adsorbents,
Water 2020, 12, 1697 5 of 11 Water 2020, 12, x FOR PEER REVIEW 5 of 11 previously reported (Mg(AlZr)-LDHs(CO or Cl) = 2.2–39 m2 g 1 and Zr-MgAl = 49 m2 g 1) adsorbents, but not of (Zr-MgAl-HT = 154 m2 g−1) [17,18].3 These results indicate− that incorporation of− Zr4+ into the but not of (Zr-MgAl-HT = 154 m2 g 1)[17,18]. These results indicate that incorporation of Zr4+ into octahedral layer of the complex nickel− -aluminum hydroxide results in an increase of the specific the octahedral layer of the complex nickel-aluminum hydroxide results in an increase of the speciﬁc surface area. surface area. Table 1. Characteristics of adsorbents. Table 1. Characteristics of adsorbents. Number of Hydroxyl Groups Specific Surface Area Adsorbents Surface pH Number of Hydroxyl Groups Speciﬁc Surface Area Adsorbents Surface pH (mmol g−11) (m22 g−11) (mmol g− ) (m g− ) NA11 7.98 1.92 22.8 NA11 7.98 1.92 22.8 NNA12A12 7 7.63.63 11.62.62 26.426.4 NNAZ1AZ1 6 6.18.18 11.08.08 51.951.9 NNAZ2AZ2 6 6.21.21 11.51.51 27.827.8
3.2. Adsorption C Capabilityapability of As(III) The quantities of As(III) adsorbed onto each each adsorbent adsorbent are are shown shown in in Figure Figure3 . 3. The The amount amount adsorbed increases increases as as NA11 NA11 << NA12NA12 < NAZ2< NAZ2 < NAZ1,< NAZ1, which which indicates indicates that thatNAZ1 NAZ1 should should be the be most the usefulmost useful for removal for removal of As(III) of As(III) from from aqueous aqueous media. media. Relationships Relationships between between the the quantity quantity of of As(III) As(III) adsorbed and the three parameters in Table 1 1 were were statisticallystatistically assessed.assessed. TheThe correlationcorrelation coecoefficientsﬃcients betwebetweenen the amount adsorbed and the surface pH, amount of hydroxyl groups, and specific speciﬁc surface area were negative 0.570, negative 0.738, and positive 0.921, respectively. Therefore, speciﬁcspecific surface area most strongly inﬂuences influences As(III) As(III) adsorption adsorption capability capability in in solution. solution. The surface properties of adsorbents are very important in the interactions with As(III) in the aqueous phase. Additionally Additionally,, the effecteﬀect of of zirconium zirconium incorporation incorporation on on the the characteristic characteristic of adsorbent of adsorbent and adsorption and adsorption capability capability of As(III) of wasAs(III) evaluated was evaluated in detail. in detail Thus,. NA11Thus, andNA11 NAZ1 and NAZ1 were selected were selected to evaluate to evaluate As(III) As(III) adsorption adsorption in the infollowing the following experiments. experiments.
1 Figure 3. 3. Amount of As(III) As(III) adsorbed. adsorbed. Initial concentration: 100 mg L L−−1,, solvent solvent volume: volume: 50 50 mL, mL, adsorbent: 0.1 g, contact time: 24 24 h, h, tem temperature:perature: 25 25 °C,◦C, agitation agitation speed: speed: 100 100 rpm. rpm. 3.3. Adsorption Kinetics 3.3. Adsorption Kinetics The kinetics of As(III) adsorption onto NA11 and NAZ1 were conducted at an initial concentration The kinetics1 of As(III) adsorption onto NA11 and NAZ1 were conducted at an initial of 100 mg L− . Adsorption equilibrium was reached within 24 h under the experimental conditions concentration of 100 mg L−1. Adsorption equilibrium was reached within 24 h under the experimental (Figure4). It is clear that adsorption of As(III) onto NA11 and NAZ1 is complicated, because the conditions (Figure 4). It is clear that adsorption of As(III) onto NA11 and NAZ1 is complicated, time to reach equilibrium would be short if the process were controlled by a single factor . Thus, because the time to reach equilibrium would be short if the process were controlled by a single factor . Thus, the adsorption mechanism was investigated by comparing results to both pseudo-first- order (2) and pseudo-second-order models (3) [28,29]:
ln(qe − qt) = lnqe − k1t, (2)
Water 2020, 12, 1697 6 of 11 the adsorption mechanism was investigated by comparing results to both pseudo-ﬁrst-order (2) and pseudo-second-order models (3) [28,29]:
Water 2020, 12, x FOR PEER REVIEW 6 of 11 ln(qe qt) = lnqe k t, (2) − − 1 t t 1 =t +t 1 (3) = + 2, (3) qt qt qe qe k2k2×qqee20 × 1 where qe and qtt areare the amounts of As(III) adsorbed (mg g−−1)) at at equilibrium equilibrium and and given given time time tt,, and k1 1 1 1 andand k2 are the pseudo-ﬁrst-orderpseudo-first-order (h(h−−1)) and pseudo-second-orderpseudo-second-order (g(g mgmg−−1 h−1−) )rate rate constants. constants. Table Table 22 showsshows the the results results of ﬁtting of fitting the experimental the experimental data to the data pseudo-ﬁrst-order to the pseudo (coe-firstﬃ-ordercient of (coefficient determination of determination= 0.817–0.961) = and 0.817 pseudo-second-order–0.961) and pseudo- (coesecondﬃcient-order of (coefficient determination of determination= 0.978–0.992) = models.0.978–0.992) The models.adsorption The of As(III) adsorption onto NA11 of As(III) and NAZ1 onto appears NA11 and to occur NAZ1 by a appears process ofto chemisorption. occur by a process The value of chemisorption.of k2 with NAZ1 The is value less than of k that2 with with NAZ1 NA11, is less which than indicates that with that NA11, As(III) which adsorption indicates is that favored As(III) at adsorptionNAZ1. This is conclusionfavored at NAZ1. is supported This conclusion by the result is supported in Figure 3by, which the result shows in Figure that a greater3, which amount shows thatof As(III) a greater is adsorbed amount by of NAZ1. As(III) Adsorption is adsorbed equilibrium by NAZ1. Adsorption also tends to equilibrium be established also more tends rapidly to be establishedusing NA11 more than NAZ1.rapidly Similarusing NA11 trends than have NAZ1. been reported Similar intrends previous have studies been reported [13,30]. Additionally,in previous studiesa previous [13, study30]. Additionally, pointed out thea previous fact that morestudy caution pointed should out the be fact exercised that more in the caution analysis should of kinetic be 2 exerciseddata . in Thus, the theanalysis chi-square of kinetic analysis data ( χ[3)1 was]. Thus, conducted the chi- forsquare the evaluation analysis (χ of2) kineticwas conducted models to for avoid the 2 evaluationincluding errors. of kine Thetic models low value to avoid of χ indicates including that errors. the kinetic The low model value ﬁts of to χ2 the indicates experimental that the data kinetic . 2 modelThe value fits to of theχ inexperimental the pseudo-ﬁrst-order data . The model value was of χ higher2 in the than pseudo that-first in the-order pseudo-second-order model was higher thanmodel that (Table in the2), pseudo which indicates-second-order that the model pseudo-second-order (Table 2), which indicates model is consideredthat the pseudo to be-second better for-order the modelobtained is considered data in this to study. be better for the obtained data in this study.
Figure 4. Eﬀect of contact time on the adsorption of As(III) using NA11 and NAZ1. Initial concentration Figure 4. Effect of contact time on the adsorption of As(III) using NA11 and NAZ1. Initial 100 mg L 1, solvent volume 50 mL, adsorbent 0.1 g, contact time 0.5, 1, 3, 6, 9, 12, 16, 20, and 24 h, concentration− 100 mg L−1, solvent volume 50 mL, adsorbent 0.1 g, contact time 0.5, 1, 3, 6, 9, 12, 16, 20, temperature 25 C, agitation speed 100 rpm, : NAZ1, : NA11. and 24 h, temperature◦ 25 °C , agitation speed •100 rpm, ●: NAZ1, ○: NA11. # Table 2. Kinetic parameters for the adsorption of As(III). Table 2. Kinetic parameters for the adsorption of As(III). Pseudo-First-Order Model Pseudo-Second-Order Model q Adsorbents e k Pseudoq -First-Order Model Pseudok -Secondq -Order Model 1 e r2 χ2 2 e r2 χ2 1 1 (g mg 1 h 1) 1 Adsorbents qe (h− k) 1 (mg gq−e ) −k2 − (mg gq− e) r2 χ2 r2 χ2 NA11 8.6 0.093−1 3.9−1 0.817 1.8 102 0.110−1 −1 9.1−1 0.978 1.8 (h ) (mg g ) × (g mg h ) (mg g ) NAZ1 14.9 6.4 6.4 0.961 2.9 10 0.066 15.2 0.992 1.4 NA11 8.6 0.093 3.9 0.817 1.8 × 102 0.110 9.1 0.978 1.8 NAZ1 14.9 6.4 6.4 0.961 2.9 × 10 0.066 15.2 0.992 1.4
3.4. Effect of pH on the Adsorption of As(III) Solution pH is a critical factor in the removal of As(III) from aqueous solution. Figure 5 shows the effect of pH on As(III) adsorption using NA11 and NAZ1. The quantity of As(III) adsorbed tends to increase with increasing pH. A similar trend using zirconium oxide-ethanolamine has been reported in a previous study . Here, solution pH tends to increase or decrease slightly after adsorption indicating that the surface of NA11 and NAZ1 may be useful as a neutralizing agent in
Water 2020, 12, 1697 7 of 11
3.4. Eﬀect of pH on the Adsorption of As(III) Solution pH is a critical factor in the removal of As(III) from aqueous solution. Figure5 shows the eﬀect of pH on As(III) adsorption using NA11 and NAZ1. The quantity of As(III) adsorbed tends to increase with increasing pH. A similar trend using zirconium oxide-ethanolamine has been reported inWater a previous2020, 12, x FOR study PEER [12 REVIEW]. Here, solution pH tends to increase or decrease slightly after adsorption7 of 11 indicating that the surface of NA11 and NAZ1 may be useful as a neutralizing agent in the wastewater treatmentthe wastewater of highly treatment acidic orof basichighly As(III) acidic samples or basic [ 12As(III),33]. Thesamples pKa,1 [1of2, H333].AsO The3 ispK 9.2,a,1 of which H3AsO indicates3 is 9.2, thatwhich As(III) indicates is a neutralthat As(III) species is a atneutral pH 9.2. species At pH at >pH9.2, 9.2. anionic At pH forms > 9.2, ofanionic As(III) forms are produced of As(III) that are undergoproduced ion that exchange undergo with ion exchange sulfate ion with from sulfate NA11 ion and from NAZ11 NA11 under and theNAZ11 experimental under the conditions experimental (see Sectionconditions 3.5). (see Section 3.5).
Figure 5. EffectEﬀect of pH on the adsorption of As(III) using NA11(NA11(A)A) and NAZ1(NAZ1(B).B). Initial concentration 1 100 mgmg LL−−1,, solvent solvent volume volume 50 50 mL, mL, adsorbent adsorbent 0.1 0.1 g, g, pH pH 2, 2, 4, 4, 6, 6, 8, 8, and and 10, 10, contact contact time time 24 24 h, h, temperature temperature 25 ◦°CC,, agitation speed 100 rpm. 3.5. As(III) Adsorption Isotherms 3.5. As(III) Adsorption Isotherms Figure6 displays adsorption isotherms of As(III) at di ﬀerent temperatures. The data provide Figure 6 displays adsorption isotherms of As(III) at different temperatures. The data provide considerable insight to the adsorptive behavior of NA11 and NAZ1 towards As(III) in aqueous considerable insight to the adsorptive behavior of NA11 and NAZ1 towards As(III) in aqueous solution. The quantities of As(III) adsorbed increase with increasing temperatures (10 < 25 < 45 ◦C), solution. The quantities of As(III) adsorbed increase with increasing temperatures (10 < 25 < 45 °C), which indicates that chemisorption is involved in the adsorption of As(III) on NA11 and NAZ1. which indicates that chemisorption is involved in the adsorption of As(III) on NA11 and NAZ1. The The solution pH was 5.5–6.4 and 5.9–6.2 for NA11 and NAZ1 in all experimental temperatures. Thus, solution pH was 5.5–6.4 and 5.9–6.2 for NA11 and NAZ1 in all experimental temperatures. Thus, the the predominant form of As(III) was not aﬀected by the temperature under our experimental conditions. predominant form of As(III) was not affected by the temperature under our experimental conditions. Langmuir and Freundlich models were applied to provide a more quantitative description of the relationship between the quantity of As(III) adsorbed and the solute concentration. The Langmuir model is described by Equation (4) :
1/q = 1/(WsaCe) + 1/Ws, (4)
1 where q is the quantity of As(III) adsorbed (mg g− ), Ws is the maximum amount of As(III) adsorbed 1 1 (mg g− ), a is the Langmuir isotherm constant (binding energy) (L mg− ), and Ce is the equilibrium 1 concentration (mg L− ). The Langmuir isotherm is applicable to monolayer coverage by the adsorbate. The Freundlich model is described by Equation (5) :
1 log q = log C + log k, (5) n
Figure 6. Effect of temperature on the adsorption of As(III) using NA11(A) and NAZ1(B). Initial concentration 1, 10, 30, 50, 70, and100 mg L−1, solvent volume 50 mL, adsorbent 0.1 g, contact time 24
Water 2020, 12, x FOR PEER REVIEW 7 of 11 the wastewater treatment of highly acidic or basic As(III) samples [12,33]. The pKa,1 of H3AsO3 is 9.2, which indicates that As(III) is a neutral species at pH 9.2. At pH > 9.2, anionic forms of As(III) are produced that undergo ion exchange with sulfate ion from NA11 and NAZ11 under the experimental conditions (see Section 3.5).
Water 2020, 12, 1697 8 of 11 where k and 1/n are the adsorption capacity and strength of adsorption, respectively. The Freundlich model describes systems where the surface of the adsorbent is heterogeneous and has sites of diﬀerent energy . Table3 shows that the Freundlich model ( 0.970) provides better correlation than the Figure 5. Effect of pH on the adsorption of As(III) using NA11(A)≥ and NAZ1(B). Initial concentration Langmuir model ( 0.965) except for NAZ1 at 25 ◦C. Previous studies have reported similar behavior 100 mg L−1, solvent≥ volume 50 mL, adsorbent 0.1 g, pH 2, 4, 6, 8, and 10, contact time 24 h, temperature using Fe-based backwashing sludge and polymer adsorbents [33,36]. The maximum adsorption 25 °C , agitation speed 100 rpm. capacity (Ws) of As(III) increases from 10 ◦C to 45 ◦C. It is worth noting that in the experimental conditions used, equilibrium data (Figure6) suggest that the plateau for maximum adsorption was 3.5. As(III) Adsorption Isotherms not reached. The maximum adsorbed amounts calculated in the Langmuir ﬁtting, however, are lower thanF someigure values6 displays measured adsorption experimentally, isotherms of which As(III) may at bedifferent due to temperatures. the use of a linearized The data equationprovide c(Equationonsiderable (4)) insight to mathematically to the adsorptive model behavior the results. of ThisNA11 indicates and NAZ1 that towards the adsorption As(III) of in As(III) aqueous on solution.NA11 and The NAZ1 quantities is an endothermic of As(III) adsorbed process, increase which waswith supported increasing by temperatures the results in (10 Figure < 25 6<. 45 In °C), the whichFreundlich indicates model, thatn ischemisorption the heterogeneity is involved factor. Therefore,in the adsorptio whenn 1/ nof= As(III)0.1–0.5, on adsorption NA11 and occurs NAZ1. easily, The solutionand when pH 1 /wasn > 2,5.5 adsorption–6.4 and 5.9 is–6.2 diﬃ forcult NA11 . and The NAZ1 values in ofall 1 e/nxperimental= 0.13 0.97 temperatures. obtained in thisThus, study the − predominantindicate that As(III)form of adsorption As(III) was onto not NA11affected and by NAZ1the temperature is favored under in aqueous our experimental solution. conditions.
Figure 6. Eﬀect of temperature on the adsorption of As(III) using NA11 (A) and NAZ1 (B). Initial Figure 6. Effect of temperature on the adsorption of As(III) using NA11(A) and NAZ1(B). Initial concentration 1, 10, 30, 50, 70, and100 mg L 1, solvent volume 50 mL, adsorbent 0.1 g, contact time 24 h, concentration 1, 10, 30, 50, 70, and100 mg L−−1, solvent volume 50 mL, adsorbent 0.1 g, contact time 24 pH 5.5-6.4 and 5.9-6.2 for NA11 and NAZ1, temperature 10 ( ), 25 ( ), and 45 C( ), agitation speed • • ◦ • 100 rpm.
Table 3. Langmuir and Freundlich constants for the adsorption of As(III).
Langmuir Constants Freundlich Constants Temperature Adsorbents W a (◦C) s 2 2 1 1 r logk 1/n r (mg g− ) (L mg− ) 10 6.1 0.02 0.965 0.1 0.91 0.970 − NA11 25 9.3 0.04 0.982 0.1 0.56 0.991 − 45 15.4 0.006 0.989 1.4 0.13 0.996 − 10 6.3 0.09 0.996 0.3 0.70 0.989 − NAZ1 25 15.3 0.01 0.935 0.4 0.97 0.768 − 45 16.6 0.10 0.977 0.29 0.54 0.999
In this study, sulfate ions are present in the interlayer of the NA11 and NAZ1 absorbents. Figure7 shows the relationship between the amount of As(III) adsorbed and the amount of sulfate ion released from NA11 and NAZ1. The correlation coeﬃcients for release from NA11 and NAZ1 are 0.797 and 0.944, respectively. The results indicate that the release of sulfate from NA11 and NAZ1 by ion exchange has a role in the adsorption mechanism of As(III). Water 2020, 12, 1697 9 of 11 Water 2020, 12, x FOR PEER REVIEW 9 of 11
Figure 7. Relationship between amount of As(III) adsorbed and amount of sulfate ion released using Figure 7. Relationship between amount of As(III) adsorbed and amount of sulfate ion released using NA11 (A) and NAZ1 (B). Initial concentration 1, 10, 30, 50, 70, and100 mg L 1, solvent volume 50 mL, NA11(A) and NAZ1(B). Initial concentration 1, 10, 30, 50, 70, and100 mg L−−1, solvent volume 50 mL, adsorbent 0.1 g, pH 10, contact time 24 h, temperature 25 C, agitation speed 100 rpm. adsorbent 0.1 g, pH 10, contact time 24 h, temperature 25 ◦°C , agitation speed 100 rpm. 3.6. Comparison of Adsorption Capability of As(III) 3.6. Comparison of Adsorption Capability of As(III) Table4 summarizes comparisons of As(III) adsorption capability of NA11 and NAZ1 with other reportedTable adsorbents 4 summarize [38s– 41comparisons]. The NAZ1 of exhibitedAs(III) adsorption a good potential capability to of be NA11 used and for removal NAZ1 with of As(III) other fromreported aqueous adsorbents media [38 compared–41]. The to NAZ1 other exhibited reported a adsorbents good potential (except to be for used drinking-water for removal treatmentof As(III) residualsfrom aqueous (WTRs)). media From compared these comparisons, to other reported NAZ1 isadsorbents expected to (except be employed for drinking in a commercial-water treatment process inresiduals the future (WTRs for As(III))). From adsorption. these comparisons, NAZ1 is expected to be employed in a commercial process in the future for As(III) adsorption. Table 4. Comparison of As(III) adsorption capacity of NA11 and NAZ1 with other reported adsorbents.
Table 4. ComparisonAdsorption of As(III) adsorption capacityInitial of NA11 and NAZ1 with other reported Temp. Contact Time Adsorbent Adsorbents Capability pH Concentration Ref. adsorbents. ( C) (h) (g/L) (mg/g) ◦ (mg/L) ZrPACM-43Adsorption 0.8 <5 50 100Initial 2Contact 13  Temp. Approximately Adsorbent AdsorbentsAl-HDTMA-sericite Capability 0.433 4.5pH -Concentration 2 Time 1  Ref. (°C) 6.7 (g/L) Iron (mg/g) (mg/L) (h) hydroxide-coated 9.0 6.6 20 0.5 7.5 135 48 1–25  ZrPACM-43 0.8 <5 × 50 − 100 2 13  alumina Silica gel Approx Al-HDTMA- impregnated with 0.4334.5 7.04.5 20–23- 12 15imately -1   sericiteferric hydroxide WTRs 15 6.0–6.5 23 375–3000 486.7 25–200  Iron hydroxideNA11- 9.3 5.5–6.4 25 100 24 2 This study NAZ19.0 15.3 5.9–6.26.6 2520 × 0.5 1007.5−135 2448 21–25 This study coated alumina Silica gel 4. Conclusionsimpregnated 4.5 7.0 20–23 1 15 -  withThe complexferric metal hydroxides NA11 and NAZ1 were prepared to study As(III) removal from hydroxide 2 1 aqueous media. The speciﬁc surface area of NAZ1 (51.9 m g− ) was greater than that of NA11 WTRs2 1 15 6.0–6.5 23 375–3000 148 25–200  (22.8 m g− ). The quantity of As(III) adsorbed onto NAZ1 (15.3 mg g− ) was also greater than that This adsorbedNA11 onto NA11 (9.39. mg3 g 1).5.5 The–6.4 correlation 25 coeﬃcient100 between the24 quantity adsorbed2 and the − study speciﬁc surface area was 0.921. The adsorption kinetics followed the pseudo-second-order model This NAZ1 15.3 5.9–6.2 25 100 24 2 (coeﬃcient of determination using NA11 and NAZ1 was 0.978 and 0.992, respectively). Adsorptionstudy isotherms data established that As(III) adsorption was an endothermic process. Ion exchange with sulfate4. Conclusions ions in the interlayer of the adsorbent was also involved in the As(III) adsorption mechanism. The complex metal hydroxides NA11 and NAZ1 were prepared to study As(III) removal from aqueous media. The specific surface area of NAZ1 (51.9 m2 g−1) was greater than that of NA11 (22.8 m2 g−1). The quantity of As(III) adsorbed onto NAZ1 (15.3 mg g−1) was also greater than that adsorbed
Water 2020, 12, 1697 10 of 11
Author Contributions: Conceptualization, N.K. and F.O.; investigation, N.N., C.S., and T.N.; resources, M.T. and M.O.; writing—original draft preparation, F.O.; writing—review and editing, F.O. and C.S.; project administration, N.K. All authors have read and agreed to the published version of the manuscript. Funding: This research was funded by The Research Foundation for Pharmaceutical Sciences. Conﬂicts of Interest: The authors declare no conﬂict of interest.
1. Transforming Our World: The 2030 Agenda for Sustainable Development. Available online: https: //sustainabledevelopment.un.org/post2015/transformingourworld (accessed on 8 May 2020). 2. Mohan, D.; Charles, P. Arsenic removal from water/wastewater using adsorbents-a critical review. J. Hazard. Mater. 2007, 142, 1–53. [CrossRef] 3. Mandal, S.; Sahu, M.K.; Patel, R.K. Adsorption studies of arsenic(III) removal from water by zirconium polyacrylamide hybrid material (ZrPACM-34). Water Resour. Ind. 2013, 4, 51–67. [CrossRef] 4. Hughes, M.F. Arsenic toxicity and potential mechanisms of action. Toxicol. Lett. 2002, 133, 1–16. [CrossRef] 5. Mandal, B.K.; Suzuki, K.T. Arsenic round the world: A review. Talanta 2002, 58, 201–235. [CrossRef] 6. Siddique, A.E.; Rahman, M.; Hossain, M.I.; Karim, Y.; Hasibuzzaman, M.M.; Biswas, S.; Islam, M.S.; Rahman, A.; Hossen, F.; Mondal, V.; et al. Association between chronic arsenic exposure and the characteristic features of asthma. Chemosphere 2020, 246, 129750. [CrossRef] 7. Paul, S.K.; Islam, M.S.; Hasibuzzaman, M.M.; Hossain, F.; Anjum, A.; Saud, Z.A.; Haque, M.M.; Sultana, P.; Haque, A.; Andric, K.B.; et al. Higher risk of hyperglycemia with greater susceptibility in females in chronic arsenic-exposed individuals in Bangladesh. Sci. Total Environ. 2019, 668, 1004–1012. [CrossRef] 8. IARC Monographs on the Identiﬁcation of Carcinogenic Hazards to Human. Available online: https: //monographs.iarc.fr/agents-classiﬁed-by-the-iarc/ (accessed on 31 May 2020). 9. Arsenic in Drinking Water. Available online: https://www.who.int/water_sanitation_health/water-quality/ guidelines/arsenic-information/en/ (accessed on 31 May 2020). 10. Vaishya, R.C.; Gupta, S.K. Modeling arsenic(III) adsorption from water by sulfate-modiﬁed iron oxide-coated sand (SMIOCS). J. Chem. Technol. Biotechnol. 2002, 89, 73–80. [CrossRef] 11. Martinson, C.A.; Reddy, K.J. Adsorption of arsenic(III) and arsenic(V) by cupric oxide nanoparticles. J. Colloid Interf. Sci. 2009, 336, 406–411. [CrossRef] 12. Mandal, S.; Padhi, T.; Patel, R.K. Studies on the removal of arsenic(III) from water by a novel hybrid material. J. Hazard. Mater. 2011, 192, 899–908. [CrossRef] 13. Ren, Z.; Zhang, G.; Paul Chen, J. Adsorptive removal of arsenic from water by an iron-zirconium binary oxide adsorbent. J. Colloid Interf. Sci. 2011, 358, 230–237. [CrossRef] 14. Ferguson, J.F.; Gavis, J. A review of arsenic cycle in natural waters. Water Res. 1972, 6, 1259–1274. [CrossRef] 15. Wu, K.; Liu, T.; Xue, W.; Wang, X. Arsenic(III) oxidation/adsorption behaviors on a new bimetal adsorbent of Mn-oxide-doped Al oxide. Chem. Eng. J. 2012, 192, 343–349. [CrossRef] 16. Ogata, F.; Nakamura, T.; Toda, M.; Otani, M.; Kawasaki, N. Evaluation of nickel-aluminum complex hydroxide for adsorption of chromium(VI) ion. Chem. Pharm. Bull. 2020, 68, 70–76. [CrossRef] 17. Ogata, F.; Ueta, E.; Kawasaki, N. Characteristics of a novel adsorbent Fe-Mg-type hydrotalcite and its adsorption capability of As(III) and Cr(VI) from aqueous solution. J. Ind. Eng. Chem. 2018, 59, 56–63. [CrossRef] 18. Zhang, X.; Guo, L.; Huang, H.; Jiang, Y.; Li, M.; Leng, Y. Removal of phosphorus by the core-shell bio-ceramic/Zn-layered double hydroxides (LDHs) composites for municipal wastewater treatment in constructed rapid inﬁltration system. Water Res. 2016, 96, 280–291. [CrossRef] 19. Radha, A.V.; Kamath, P.V. Aging of trivalent metal hydroxide/oxide gels in divalent metal salt solutions: Mechanism of formation of layered double hydroxides (LDHs). Bull. Mater. Sci. 2003, 26, 661–666. [CrossRef] 20. Ogata, F.; Nagai, N.; Toda, M.; Otani, M.; Nakamura, T.; Kawasaki, N. Evaluation of the interaction between borate ions and nickel-aluminum complex hydroxide for puriﬁcation of wastewater. Chem. Pharm. Bull. 2019, 67, 487–492. [CrossRef] Water 2020, 12, 1697 11 of 11
21. Wu, P.; Xia, L.; Liu, Y.; Wu, J.; Chen, Q.; Song, S. Simultaneous sorption of arsenate and ﬂuoride on calcined Mg-Fe-La hydrotalcite-like compound from water. ACS Sustain. Chem. Eng. 2018, 6, 16287–16297. [CrossRef] 22. Chitrakar, R.; Tezuka, S.; Sonoda, A.; Sakane, K.; Ooi, K.; Hirotsu, T. Synthesis and phosphate uptake behavior of Zr4+ incorporated MgAl-layered double hydroxides. J. Colloid Interf. Sci. 2007, 313, 53–63. [CrossRef] 23. Miyauchi, H.; Yamamoto, T.; Chitrakar, R.; Makita, Y.; Wang, Z.; Kawai, J.; Hirotsu, T. Phosphate adsorption site on zirconium ion modiﬁed MgAl-layered double hydroxides. Top Catal. 2009, 52, 714–723. [CrossRef] 24. Ogata, F.; Iijima, S.; Toda, M.; Otani, M.; Nakamura, T.; Kawasaki, N. Characterization and phosphate adsorption capability of novel nickel-aluminum-zirconium complex hydroxide. Chem. Pharm. Bull. 2020, 68, 292–297. [CrossRef] 25. Ymashita, T.; Ozawa, Y.; Nakajima, N.; Murata, T. Collection of uranium from sea water with hydrous oxide adsorbents. 1. Ion exchange properties and uranium adsorption of hydrous titanium(IV) oxide. Nippon Kagaku Kaishi 1978, 8, 1057–1061. [CrossRef] 26. Ogata, F.; Ueta, E.; Toda, M.; Otani, M.; Kawasaki, N. Adsorption of phosphate ions from an aqueous solution by calcined nickel-cobalt binary hydroxide. Water Sci. Technol. 2017, 75, 94–105. [CrossRef] 27. Türk, T.; Alp, I.˙ Arsenic removal from aqueous solutions with Fe-hydrotalcite supported magnetite nanoparticle. J. Ind. Eng. Chem. 2014, 20, 732–738. [CrossRef] 28. Lagergren, S. Zur theorie der sogenannten adsorption geloster stoﬃe, Kunglia Svenska Vetenskapsakademiens. Handlingar 1898, 24, 1–39. 29. Ho, Y.S.; McKay, G. Pseudo-second order model for sorption process. Pro Biochem. 1999, 34, 451–465. [CrossRef] 30. Raven, K.P.; Jain, A.; Loeppert, R.H. Arsenite and arsenate adsorption on ferrihydrite: Kinetics, equilibrium, and adsorption evelopes. Environ. Sci. Technol. 1998, 32, 344–349. [CrossRef] 31. Simonin, J.P. On the comparison of pseudo-ﬁrst order and pseudo-second order rate laws in the modeling of adsorption kinetics. Chem. Eng. J. 2016, 300, 254–263. [CrossRef] 32. Ho, Y.S. Selection of optimum sorption isotherm. Carbon 2004, 42, 2115–2116. [CrossRef] 33. Wu, K.; Liu, R.; Li, T.; Liu, H.; Peng, J.; Qu, J. Removal of arsenic(III) from aqueous solution using a low-cost by-product in Fe-removal plants-Fe-based backwashing sludge. Chem. Eng. J. 2013, 226, 292–401. [CrossRef] 34. Langmuir, I. The constitution and fundamental properties of solids and liquids. J. Am. Chem. Soc. 1916, 38, 2221–2295. [CrossRef] 35. Freundlich, H.M.T. Over the adsorption in solution. J. Phys. Chem. 1906, 57, 385–471. 36. Li, H.T.; Xu, M.C.; Shi, Q.; He, B.L. Isotherm analysis of phenol adsorption on polymeric adsorbents from nanoaqueous solution. J. Colloid. Interf. Sci. 2004, 271, 47–54. [CrossRef] 37. Abe, I.; Hayashi, K.; Kitagawa, M. Studies on the adsorption of surfactants on activated carbons. I. Adsorption of nonionic surfactants. Yukagaku 1976, 25, 145–150. 38. Tiwari, D.; Lee, S.M. Novel hybrid materials in the remediation of ground waters contaminated with As(III) and As(V). Chem. Eng. J. 2012, 204-206, 23–31. [CrossRef] 39. Hlavay, J.; Polyak, K. Determination of surface properties of iron hydroxide-coated alumina adsorbent prepared for removal of arsenic from drinking water. J. Colloid Interf. Sci. 2005, 284, 71–77. [CrossRef] 40. Yoshida, I.; Kobayashi, H.; Ueno, K. Selective adsorption of arsenic ions on silica gel impregnated with ferric hydroxide. Anal. Lett. 1976, 9, 1125–1133. [CrossRef] 41. Makris, K.C.; Sarkar, D.; Datta, R. Evaluating a drinking-water waste by-product as a novel sorbent for arsenic. Chemosphere 2006, 64, 730–741. [CrossRef]
© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).